# Predicting Ignition Time Under Transient Heat Flux Using Results

```48
6.4 Heat Release Rate
~50kWlmT
; -~-. 35 kWlm2
20 kWlm2
O~I
o
__________
60
~
____________ _____________________________
~
120 180 240 300 360 420 480 540 600 660 720 780 840 900 960 1020 1080 1140 1200 1260 1320
,Time (sec)
Figure 6.15: Heat Release Rates for Tawa
The heat release characteristics displayed in Figure 6.15 allow the calculation of how
much heat the material will emit when it is involved in combustion. This value is
called the effective heat of combustion (MJ/kg).
Figure 6.14 shows the plot of the heat release rate over the test period. As can be seen
there are two peaks in the data collected. The first peak is due to ignition. Prior to
ignition there is a build up of combustible gases above the surface of the sample.
When ignition occurs, these gases are able to combust. These gases are consumed in
the combustion reaction and the heat release rate drops to a steady state level.
The second peak is related to the temperature profile through the wood sample. As
the temperature within the sample increases, more volatiles are given off. The surface
has charred during the test and, at the stage where the heat release rate begins to
increase, the surface allows the rapid movement of pyrolyzates to the surface reaction
zone. Therefore, there is an increase in the mass loss rate as the consumption of fuel
increases to maintain the increasing heat release rate. This characteristic is confirmed
--------.----.~-~
49
by Figure 6.16. The mass loss rate increases in conjunction with the increase in the
heat release rate.
30~-
______.____________________________________________
~
25
20
10
5
o
Time (see)
Figure 6.16: Mass Loss Characteristics for Tawa
Figure 6.16 shows that for each test the mass loss rate increases after a period of
approximately 600 seconds after ignition. This time corresponds to the beginning of
the increase in the heat release rate toward the second peak ..
An interesting occurrence in Figure 6.15 is that the maximum heat release rate for the
test at 20 kW/m2 is greater than that for the 50 kW/m2 test. The expected relationship
would be that the heat release rate would be greatest for the higher fluxes and would
decrease as the level of incident heat flux decreased, as a more intense fast burning
fire would be expected at a higher flux level. This occurrence was also noted in other
materials tested, most notably Radiata Pine.
```